UNIVERSITI TEKNIKAL MALAYSIA MELAKA (UTeM)
INFLUENCE OF SOLUTION PROCESS PARAMETER TO
COBALT CATALYST THIN FILM AND PARTICLE FORMATION
This report is submitted with requirement of the Universiti Teknikal Malaysia Melaka
(UTeM) for the Bachelor Degree of Manufacturing Engineering (Engineering Materials)
NIK MOHAMAD AZREN BIN MOHD ZUBIR
FACULTY OF MANUFACTURING ENGINEERING
INFLUENCE OF SOLUTION PROCESS PARAMETER TO
COBALT CATALYST THIN FILM AND PARTICLE
NIK MOHAMAD AZREN BIN MOHD ZUBIR
UNIVERSITI TEKNIKAL MALAYSIA MELAKA
I hereby, declared this report entitled ‘Influence of Solution Process Parameter to Cobalt
Catalyst Thin Film and Particle Formation’ is the results of my own research except as
cited in references.
Signature : ………
Author’s Name : Nik Mohamad Azren Bin Mohd Zubir
This report is submitted to the Faculty of Manufacturing Engineering of UTeM as a
partial fulfillment to the requirements for the degree of Bachelor of Manufacturing
Engineering (Engineering Materials) (Hons.). The member of the supervisory is as
This report study about the influence of solution process parameter to cobalt catalyst thin
film and particle formation. Cobalt is selected as the choice of material due to its
excellent performance to produce thin film with thickness below 100 nm. There are two
phase involved during thin film preparation which are spin coating and annealing. Using
spin coating process the thickness of the film can be manipulated by changing its spin
speed or altering solution viscosity. In annealing process the thin film is heat treated in
order to produce uniform size of cobalt particles in thin film. Furthermore after
completing these two phase in solution process, the cobalt thin film will undergo
characterization for surface morphology and elemental confirmation that can be done by
using Field Emission Scanning Electron Microscopy (FE-SEM) and Xray Diffraction
(XRD).The result shows that increasing spin speed reduces the Co film thickness and
increasing temperature of heat treatment result in larger particle formation. This can be
concluded that particle and thin film formation was successfully done by using solution
Laporan ini mengkaji mengenai pengaruh parameter proses larutan keatas pembentukan
partikel untuk kobalt sebagai pemangkin filem nipis. Cobalt telah dijadikan sebagai
bahan pilihan disebabkan oleh prestasinya yang cemerlang dalam menghasilkan filem
nipis dengan ketebalan kurang daripada 100 nm. Terdapat dua fasa yang terlibat semasa
penyediaan filem nipis iaitu lapisan putaran dan sepuh lindap. Menggunakan proses
salutan spin ketebalan filem itu boleh dimanipulasi dengan menukar kelajuan putaran
atau mengubah kelikatan larutan. Dalam proses penyepuh lindapan filem nipis
dikenakan rawatan haba untuk menghasilkan saiz zarah kobalt yang seragam dalam
filem nipis. Tambahan pula selepas menamatkan kedua-dua fasa dalam proses larutan,
filem kobalt nipis akan menjalani pencirian untuk morfologi permukaan dan pengesahan
unsur. ia boleh dilakukan dengan menggunakan Mikroskop Transmisi Elektron (TEM),
Field Mikroskop Pelepasan Imbasan Elektron (FE SEM) dan Difraksi Xray (XRD). Hasilnya menunjukkan bahawa peningkatan kelajuan putaran mengurangkan ketebalan
filem Co dan suhu yang semakin meningkat hasil rawatan haba dalam pembentukan
zarah yang lebih besar. Ini boleh membuat kesimpulan bahawa zarah dan filem nipis
To my parents and family members for their continuous support throughout my study.
To my supervisor and postgraduate student for their advice and guidance in completing
First of all, I would like to express my gratitude to Allah the Almighty for giving me the
health to complete my Final Year Project. I would like to thank both my parents and my
family for their continuous support and help in many ways and aspects in order to
complete my research. I would also like to thank my supervisor, Dr Mohd Asyadi Azam
Bin Mohd Abid and the postgraduate student who willing to spare their time in guiding
and share their experiences for me to complete this project. Without their help, I would
not be able to complete this research on time and with good contents.
I would also like to thank all my friends who have support and willing to help me
whenever I faced any problem in completing the research and the report.
Last but not least, I would like to thank all the lab technicians for all their help in
completing this project. Without their help, I will facing many difficulties in order to
List of Abbreviations, Symbols and Nomenclature xi
CHAPTER 1 : INTRODUCTION 1
2.2.1 Thin Film Deposition Technique 7
2.3 Spin Coating 8
2.3.1 Working Principle 8
2.3.2 Influence of Solution Process Parameter on Thin Film Thickness 10 18.104.22.168 Spin Coating Speed 10
22.214.171.124 Spin Time 11
126.96.36.199 Precursor Concentration 12 188.8.131.52 Evaporation Rate of Solvent 13
2.4 Precursor Solution 14
2.5 Metal Catalyst Thin Film 14
2.5.1 Cobalt Catalyst Particles 15
2.6.1 Grain Growth Process during Annealing 17 2.6.2 Experiment Condition of Annealing 17 2.6.3 Influence of Annealing Temperature on Film Microstructure 19
CHAPTER 3 : METHODOLOGY 20
3.1 Flowchart of Methodology 21
3.1.1 Cleaning and Solution Preparation 22
184.108.40.206 Substrate Cleaning 22
220.127.116.11 Precursor Solution Preparation 22
3.1.2 Thin Film Preparation 23
3.2 Machine And Apparatus 24
3.3.1 Field Emission Scanning Electron Microscopy (FE-SEM) 27
3.3.3 X-Ray Diffraction (XRD) 28
CHAPTER 4 : RESULTS AND DISCUSSION 29
4.1 Chemical reaction during thin film formation of Co3O4. 30 4.2 Effect of Aging Time on Structural Properties of Cobalt Thin Film 33 4.3 Effect of Spin Speed on Thin Film Thickness 34 4.4 Effect of Heat Treatment Temperature on Particle Formation 41
CHAPTER 5 : CONCLUSION AND RECOMMENDATION 48
5.1 Conclusion 48
5.2 Recommendation 48
5.3 Future Prospect 49
LIST OF TABLE
LIST OF FIGURES
2.1 Carbon nanotube structure 6
2.2 Overall stages in spin coating process mechanism
(source: Aguilar et al.,2011) 8 2.3 Influence of spin speed on film thickness
(sources: Alvankarian et al. 2012) 10 2.4 Influence of spin time on film thickness
( source :http://www.elveflow./microfluidic-reviews-and
tutorials/pdmsmembrane-thickness-of-a-spin-coated-pdms-layer) 11 2.5 Influence of precursor concentration on film thickness
(source: Shivaraj et al., 2013) 12 2.6 Influence Evaporation rate of solvent on PMMA film thickness
(source: Haas et al., 2000) 13 2.7 (A) - (D) annealed in air flow at 500 oC and (E) - (H) annealed by
vacuum at 500°C (source: Wei et al., 2009 ) 18 2.8 AFM image show cobalt particle formation on different annealing
temperature (A) before annealing,(B) 600°C (C) ,700°C and
4.13 FESEM micrograph (A) and average particle of cobalt thin film (B)
for 450 °C 42
4.14 FESEM micrograph (A ) and average particle of cobalt thin film (B)
for 500 °C 43
4.15 FESEM micrograph (A ) and average particle of cobalt
thin film (B ) for 550 °C 44
4.16 FE-SEM micrograph (A) and average particle of cobalt thin film
(B ) for 600 °C 45
FE-SEM - Field Emission Scanning Electron Microscopy ISFM - International Symposium Functional Material ITEX - Invention Innovation and Technology Exhibition kV - kilo Voltage
MWCNT - Multi Walled Carbon nanotube nm - nanometer
PtMn - Platinum Manganese PVD - Physical Vapor Deposition RFID - Radio Frequency Identification rpm - Revolution Per Minutes
s - Second
Sdn. - Sendirian
SiGe - Silicon Germanium
SWCNT - Single -Walled Carbon nanotube TEOS - Tetraethyl Orthosilicate
TiW - Titanium Tungsten
can affect the thin film formation . Cobalt is used as the material for the thin film that acted as catalyst for CNT growth. This chapter described about the relevance and background to the project, it discussed about the importance of thin film towards CNT growth. Several objectives and scope that needed to be achieved in this project is briefly explained .
attention due to its simple deposition procedure, easy control of chemical components and low cost preparation to obtain high quality thin films (Shivaraj et al., 2013).
Spin coating technique is one of the methods involved in solution process technique to deposit thin film. The properties of thin film deposited by spin coating technique are influenced by several parameters such as pre coating, coating, and post coating parameter (Shivaraj., 2013). Spin coating is consists of several stages which are deposition, spin up, spin off and evaporation. During spin coating, A fluid resin is deposited at the centre substrate and spinning the substrate at high speed. Centrifugal force will cause the resin to spread over the planar on the substrate and leaving a thin film of resin on the surface. Final uniform thickness is influenced by several parameters such as spinning speed, spinning duration, solvent concentration, volume of the resin, drying rate etc.
1.2 Problem Statement
In CNTs production, the application of physical vapour deposition (PVD) method is widely used to produce thin film which is a layer that contains catalyst nanoparticles. The catalyst is acted like seeds that enable the growth of CNT. Unfortunately, the needs of large vacuum device in PVD has led to inefficiency usage of energy and material in manufacturing process and consumes higher production cost. In PVD large amount of heat is required which it needs the skilful operator. Furthermore the rate of coating is slow even though it provide good particle formation thin film thickness.
film and particle formation through spin coating process and heat treatment. However, there are still few studies on solution process to achieve optimum parameter that can be selected in order to provide good thin film formation for CNT growth. In order to achieve optimum parameter, consistency and repeatability of the result is required.
The main purpose for this project is to produce and characterize the cobalt catalyst thin film. In order to reach the goals, the research is conducted based on several aims which are:
1. To investigate the effect of spin coating speed parameter to produce uniform thickness of cobalt catalyst thin film.
2. To study the influence of heat treatment of thin film for Co nanoparticles formation.
This research will be based on several scopes to ensure that the project will not be distracted by other factors.
To achieve the first objective ,the parameter and scope will be covered on :
1. Cobalt acetate tetrahydrate and ethanol is used to form precursor solution cobalt acetate precursor.
For the second objective, the scope covered is :
1. The heat treatment is done on vacuum furnace for 10 minutes for all temperature parameter.
2. The range of heat treatment temperature range from 450 °C to 600 °C.
5 consuming PVD to the solution process which can be conducted in a simple way in ambient environment. This chapter provides background information and history about CNT. Information on particle synthesis and its link to the catalytic growth on particles is also provided. Moreover theory and information about particles and particle synthesis is discussed and elaborated. Furthermore, several types of thin film deposition that is often from the previous research. Finally influence of parameter of spin coating and annealing are also described.
2.1 Carbon Nanotubes (CNTs)
CNTs were first discovered about 30 years ago. However during that time CNTs are not appreaciated.Then, in 1950s, Rogwer Bacon discovered a new strange type of carbon. He found that hollow tubes of carbon consist of graphite layers separated in the same spacing as the planar layer of the graphite. later in 1970s Morinobu Endo found that there are some tube consist of a single layer roll of graphite. In 1991 Sumio Ijima found an extremely thin needle like material during examination of carbon material under electron microscope. Later he named the strucure as CNTs.
structure such as diameter and the chirality. The tube can be made into Single-Walled Carbon Nanotube (SWCNT) and Multi-Single-Walled Carbon Nanotube (MWCNT). SWCNT is the tube that is made out of single layer carbon atom. The CNTs can posses metallic or semiconductor ability depending on their geometric structure such as diameter and the chirality. Multi-walled Carbon Nanotube (MWCNT) consists of layers of carbon sheets that wrapped one another. Several method have known in order to produce CNTs such as laser ablation, arc dicharge deposition and chemical vapor deposition.
Figure 2.1: Carbon nanotube structure
2.2 Thin Film
2.2.1 Thin Film Deposition Technique
Physical Vapour Deposition (PVD) is a technique that forms thin layer of chemicals is applied on substrates which are later vaporized with heat in a vacuum chamber. It is suitable to fabricate films with thicknesses in the range of a few nanometres to thousands of nanometres film . Besides that, production of multilayer coatings, graded composition deposits, very thick deposits and free standing structures are possible when using PVD.
Furthermore, the advantages of PVD are it can provide high deposition rate with less surface damage of thin film and produce excellent purity of the film due to vacuum mechanism (Maltone, 2009). However it is difficult to control film composition while maintaining uniform film thickness when using vacuum evaporation method .There are three types of processing method in PVD which are vacuum evaporation, sputtering deposition and ion plating .
2.3 Spin Coating
Spin coating is one of the techniques in sol gel process. It has been used for several decades for the application of thin films. It is a typical process that involves depositing a small puddle of a fluid resin onto the centre of a substrate and then spinning the substrate at high speed (Taleb et al., 2009). The spin coating technique
is a fast and easy method to generate thin film out of the solutions (Aguilar et al.,
2011). It is also able to apply uniform thin films to flat substrates. In this process a solution will be deposited on the substrate and rotated at high speed in order to spread the fluid by centrifugal force.
2.3.1 Working Principle
Based on Figure 2.1 , the mechanism of the spin can be divided into four stages which are deposition, up, off and evaporation of solvent. During the spin-off stage and evaporation stage, they are usually overlapped since both run simultaneously (Sahu et al., 2009).